Crystal structure, coloring problem and magnetism of Gd(5-x)Zr(x)Si4.
Yao, Jinlei; Lyutyy, Pavlo; Mozharivskyj, Yurij; Dalton transactions (Cambridge, England : 2003) 40 (2011) 4275–4283; doi:10.1039/c0dt01821j

data_7015687
_publ_section_title
;
 Crystal structure, coloring problem and magnetism of Gd(5-x)Zr(x)Si4.
;
_journal_issue                   16
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              4275
_journal_page_last               4283
_journal_paper_doi               10.1039/c0dt01821j
_journal_volume                  40
_journal_year                    2011
_chemical_formula_sum            'Gd4.42 Si4 Zr0.58'
_chemical_formula_weight         860.15
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.4125(5)
_cell_length_b                   14.5742(9)
_cell_length_c                   7.6693(5)
_cell_measurement_reflns_used    1157
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.20
_cell_measurement_theta_min      3.00
_cell_volume                     828.52(9)
_computing_cell_refinement       X-Area
_computing_data_collection       X-Area
_computing_data_reduction        X-Red32
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'STOE IPDSII'
_diffrn_measurement_method       'omega scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0438
_diffrn_reflns_av_sigmaI/netI    0.0285
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            8292
_diffrn_reflns_theta_full        29.20
_diffrn_reflns_theta_max         29.20
_diffrn_reflns_theta_min         3.00
_exptl_absorpt_coefficient_mu    36.056
_exptl_absorpt_correction_T_max  0.6521
_exptl_absorpt_correction_T_min  0.0907
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   X-Red
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    6.896
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Plate
_exptl_crystal_F_000             1448
_exptl_crystal_size_max          0.138
_exptl_crystal_size_mid          0.062
_exptl_crystal_size_min          0.012
_refine_diff_density_max         0.796
_refine_diff_density_min         -1.136
_refine_diff_density_rms         0.229
_refine_ls_extinction_coef       0.00084(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.933
_refine_ls_matrix_type           full
_refine_ls_number_parameters     49
_refine_ls_number_reflns         1157
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.933
_refine_ls_R_factor_all          0.0275
_refine_ls_R_factor_gt           0.0169
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0036P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0184
_refine_ls_wR_factor_ref         0.0194
_reflns_number_gt                994
_reflns_number_total             1157
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c0dt01821j.cif
_cod_data_source_block           pnma_Gd4.42Zr0.58Si4
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Orthorhombic' changed to 'orthorhombic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1555 2011-01-17 13:19:09Z saulius 
;
_cod_original_sg_symbol_H-M      Pnma
_cod_database_code               7015687